Molecular Size and Solvation of Low Molecular Weight Poly( ethylene Oxide) and
Phenol-Formaldehyde Resols in Different Solvents
BERNARD RIEDL and M.-J. VOHL, Dkpartement des Sciences du Bois, Centre de Recherche en Sciences et en Ingknikrie des
Macromoldcules, Universiti Laval, St.-Foy, QC, Canada GlK 7P4, and LOUIS CALVE, Forintek COT, 800 Chemin Montr6a1,
Ottawa Canada K l G 325
Several solvent systems are presently used to characterize the molecular weight of phenol-for- maldehyde resins. However, results reported in the literature for different molecular weights may not be representative of true molecular weight, but rather may be distorted by aggregation and solvation. In this report an effort to clarify this situation was conducted, first by using a suitable calibration with poly(ethy1ene glycol) and then using this polymer as a molecular size standard to determine the size of phenol-formaldehyde oligomers in solution. In the calculation of the molecular sizes of phenol-formaldehyde resols, proper accounting of the variation of the Mark-Houwink parameters with molecular weight for low degrees of polymerization must be made for poly(ethy1ene glycol). The Mark-Houwink constants for poly(ethy1ene glycol) are very similar in presence or absence of salts, and are considered to be unaffected by solution ionic strength. It is not the case for phenol-formaldehyde, whae apparent molecular size varies with the nature of the solvent. The actual molecular weight and molecular dimension distribution are discussed for different type A resols used as adhesives in the wood composite industry.
Several solvent systems are used to characterize the molecular weight (MW) of phenol-formaldehyde (PF) resins. Results reported in the literature may not be representative of true molecular weight, but are distorted by aggrega- tion and solvation.',' This is also true for lignin, the naturally occurring polymer, which is a partially degraded (when solvated), crosslinked p~ lymer ,~ p~lyacrylonitrile,~ and other polymer^.^ We wish to report on an effort to clarify this situation, by using suitable calibrations with low molecular weight poly(ethy1ene oxide), also known as poly(ethy1ene glycol) or PEG. This poly- mer was used as a molecular size standard to determine the size of PF molecules in solution in the presence of salts. PEG was chosen as the reference polymer since very low molecular weights are available: however, proper care must be taken in establishing the molecular weight-intrinsic viscosity (log-log) curve, since i t is nonlinear, especially a t low molecular weights. This calibra- tion must be conducted for each solvent system characterized, as the use of Mark-Houwink (MH)6 parameters K and a only is not accurate enough at low molecular weights.
Journal of Applied Polymer Science, Vol. 39, 341-353 (1990) 0 1990 John Wiley & Sons, Inc. CCC 0021-8995/90/020341-13$04.00
342 RIEDL, VOHL, AND CALVE
The use of solvent with adjusted ionic strengths have been useful in measuring the molecular weight distribution of aggregating polymers in solu- t i ~ n . ~ In general the effect of salts (ionic strength) on the solvation of PEG is limited, as is indicated by the similarity of MH parameted in tetrahydrofu- ran (THF), n, n-dimethylformamide (DMF), and water, on the one hand, and, on the other hand, as will be shown, ionic solutions such as THF with 0.4% trichloroacetic acid (TCAA), DMF with 0.1M lithium chloride (LiCl), and water-borax-NaOH (pH 10) buffer. These solvent/cosolvent systems were chosen for their ability to solubilize res~ls.~-' For the resols, the molecular solvation in these different solvent systems is quite different, as will be shown. The determination of the intrinsic viscosity and the value of the MH con- stants for PEG is required to determine the molecular size distribution of the resols, and to help determine the degree to which aggregation or association in solution exists.
To compare the performance of different columns/solvent systems, it is especially convenient to convert MW distributions to ([ T J ] * M ) distribution and averages, where M is the molecular weight, [ 171, the intrinsic viscosity and ([TI* M ) corresponds to molecular size. Rudin and Hoegy'O showed that universal calibration is possible for relatively low molecular weights without correction for concentration effects. It is then possible to obtain molecular weight averages as well as molecular size averages in the aforementioned solvents. If there is no aggregation, the calculated molecular weight and size distribution of two resols should give the same averages as the experimentally determined distribution for the mixture of both.
The aim of such research is to characterize in a nonambiguous manner the molecular size distribution of resols used as adhesives in the wood composite industry and to eventually correlate these data with kinetic, spectroscopic, and mechanical results to obtain better, low-cost resol systems. For instance, it is not known which molecular size distribution of resol provides the best adhesive properties when used alone or combined with specific wood waste extenders or the relationship between molecular size distribution and the curing parameters.
Detailed descriptions of the size-exclusion chromatography (SEC) columns and solvent systems used to characterize the resols are given in Ref. 11. In summary, size exclusion chromatography was conducted on phenol-for- maldehyde resols, with prior PEG calibration on the following column/solvent systems: (1) Ultrastyragel (Waters) 100 and 500 A columns in series a t 25C with THF/O.4% TCAA as solvent, (2) PLgel (Polymer Laboratories, U.K.) 50 and 500 A columns in series with DMF as solvent a t 25"C, and (3) same as (2) with DMF/O.lM LiCl as solvent at 25 and 85C. Once the columns have been exposed to high ionic strength solvents, it has been found out that it is best not to return the columns to pure solvents, since the nonmobile phase is sensitive to ionic strengths changes, i.e., these columns should be kept for SEC of resols. Measurements were also made with Ultrahydrogel (Waters) 120 and 500 A columns in series with water-borax-NaOH pH 10 buffer12; however, the resulting SEC spectra were indicative of an interference due to specific
LOW MW POLY(ETHYLENE OXIDE) AND PF RESOLS
1, -I 100 1000 1 E4 1 E5
Molecular weight (g-rnol-l)
50 100 1000 1 E4 1 E5 Molecular weight (g-rnol-)
100 1000 1 E4 1 E5
Molecular weight (g-mol-)
Fig. 1. Intrinsic viscosities [ q ] of poly(ethy1ene glycol) as a function of the weight average molecular weight for the different solvent systems: (0) in the pure solvent; (0) in mixed solvent. (A) Tetrahydrofuran and tetrahydrofuran with 0.4% trichloroacetic acid; (B) water14 and water-NaOH pH 10 buffer; (C) n, n-dimethylformamide and n, n-dimethylformamide with 0.1M lithium chloride.
344 RIEDL, VOHL, AND CAL-
TABLE I Mark-Houwink Constants (A, K, a) for the Low Molecular Weight
PEG in Different Solvent Systems, as Well as Constants (A, B, C) for the Mark-Houwink Curves
A K' Number of Solvent system (cm3 g-') aa Ab Bb Cb data points'
THF, 25C 1.4 0.020 0.73 0.265 -0.251 0.123 7 THF/TCAA, 25C 1.2 0.014 0.79 0.151 -0.212 0.125 7 Water, 25"Cd 1.5 0.029 0.72 Water/borax-
DMF 25C" 2.0 0.024 0.73 NaOH buffer, 25C 2.2 0.013 0.82 0.940 -0.589 0.176 6
DMF/O.lM LiCl, 25C 1.2 0.032 0.70 -0.165 0.036 0.083 4
'Calculated from the slope at MW = lo4. bConstants of the equation log[q] = A + B log(M) + C log(M)2. 'For MW range, see Figures la-c. dData from Ref. 14. eData from Ref. 15.
interactions of the column gel with PF resols and thus were not usable. The experimental setup consisted of a Waters WISP 710B injection system, M45B pump, R401 differential refractometer, and programmable system controller with data module.
The intrinsic viscosities of poly(ethy1ene oxide) oligomers used were mea- sured in THF, THF/OA% TCAA, water-borax-NaOH pH 10 buffer and DMF/O.lM LiCl (no measurements were made in DMF/LiCl a t 85C). The weight average molecular weights of the oligomers were, with the polydispersi- ties in parentheses, 215(1.06), 415(1.14), 620(1.18), 1000(1.15), 3000(1.09), 8000(1.58), and 14,000(1.24) as measured with Ultrastyragel (Waters) 100 and 500 A columns in THF, calibrated with PEG standards (Polymer Laborato- ries) whose polydispersities were between 1.00 and 1.11. The PEG of molecular weight 100,OOO (Polysciences) was used as such. The LiCl (Mallinckrodt) and TCAA (BDH) were reagent grade and the DMF and THF (Aldrich) were HPLC grade.
The viscosities were measured in an Ubbelohde (Industrial Research Glass- ware Co) viscosimeter at 25C. The resulting intrinsic viscosities are shown in Figure 1 and the corresponding MH constants in Table I.
RESULTS AND DISCUSSION
Poly(ethy1ene Glycol) Molecular Size in Solution
Poly(ethy1ene glycol), as several other ~olymers, '~ does not follow a linear Mark-Houwink relationship, such as
 = K'M" (1) where K' is the Huggins constant, M the molecular weight, and a the exponent (sometimes symbolized as a), when the logarithm of the intrinsic viscosity is plotted, as a function of the logarithm of the weight average molecular weight [Figs. l(a)-l(c)]. Instead, the curve has a distinct upward
LOW MW POLY(ETHYLENE OXIDE) AND PF RESOLS 345
concavity at low molecular weights, ie, the Huggins constant K is higher, and the exponent (Y lower than in the high (> 1OOO) molecular weight linear region.13-16 In fact, a tends toward 0.5, at very low molecular weights for the ethylene glycol oligomers. The value of the exponent a may even reach 0.5 or a lower value for other polymers, although the oligomer is not in an ideal 0 solvent: This is possible because small chains do not obey the same long range statistics as large chains.16 Also, branching lowers the value of a in a 8 solvent, (typical value is 0.25 for a highly branched ~olymer'~). Low molecular weights resols would be expected to be highly branched since one of the monomers, phenol, is trifunctional.
Sadron and Rempp18 used the simple empiric equation
to represent the variation of [q] with MW, for linear low molecular weight polymers, where A is a constant which becomes negligible at high molecular weight. In this particular case, K and (Y were calculated from the slope and intercept of the curve of the logarithm [q] as a function of the logarithm of the molecular weight as expressed in eq. (5) at relatively high molecular weight (lo4), and the value of the parameter A was then obtained by least squares from the low molecular weight data. Table I gives the values for A, K , and a for PEG in THF, water, and DMF: the difference between the MH parameters for these solvents is small in view of the high variation of K and (Y with solvent nature [and temperature, especially in water6] as seen in Figure 2, where K is shown as a function of a: This type of representation is called an Elias plot,6*'9*20 where K is seen to be inversely proportional to a.
P 4 2 4l (v 0 7
1 -carbon tetrachloride 2 -TH F
3-THF/TCM 4- WATER
5- WATER/BORAX 6-DMF
7- DM F/UC I
O ! I I I I 0.500 0.600 0.700 0.800
a Fig. 2. Mark-Houwink constants K vs. a (Elias plot) for high (> 1ooO) molecular weight
poly(ethy1ene glycol) for the different solvent systems: (1) carbon tetrachloride"; (2) tetrahydro- furan; (3) tetrahydrofuran with 0.4% trichloroacetic acid; (4) water14; (5) water-NaOH pH 10 buffer; (6) n, n-dimethylf~rmamide'~; (7) n, n-dimethylformamide with 0.1M lithium chloride.
346 RIEDL, VOHL, AND CALVE
Values of 0.12 cm3 g-' for K and 0.5 for a indicate an ideal (e.g., poor) solvent, while values of 0.020 cm3 g-' for K and 0.8 for a indicate a good solvent. Carbon tetrachloride would then be a mediocre solvent and the other afore- mentioned solvents would all be rather good solvents.
The salting out of PEG is related to the order of increased effective hydrated radii,lg and as such LiCl has very little effect on the LCST of PEG.lg The effect of TCAA in THF, borax-NaOH in water, and LiCl in DMF on the hydrodynamic volume of PEG is negligible a t molecular weights above lo4 and only slight for PEG oligomers [Figs. l(a)-l(c)]. The addition of TCAA to THF (Fig. 2, points 2-3) and of borax-NaOH (Fig. 2, points 4-5) to water slightly increases the value of a, while the addition of LiCl to DMF decreases a. As seen in Figure 2, these changes are not very great, compared to the effect of different solvents (CC1,) or temperatures: for instance, a is about 0.81 in water at 45C.6
Phenol-Formaldehyde Resol Molecular Size in Solution
In the literature, molecular weight distributions for resols are usually expressed in terms of retention times or (occasionally) molecular weights, relative to a calibration p ~ l y m e r . ~ - ~ * ~ ~ ~ 22 Ho wever, PF resols may be swollen in different manners in different solvents according to their interaction with the solvent. Moreover, the polymer used for column calibration will also be affected similarly. In order to take these effects into account, the size of the polymer were characterized through the hydrodynamic volume, rather than the molecular weight, using the expression
[ q ] * M = M * ( A + KM") (3) which corresponds to that given by universal c a l i b r a t i ~ n ~ ~ ~ ~ ~ ~ ~ since, in SEC, the hydrodynamic volume determines the retention times. [ q] * M has the dimensions of cm3 mol-' and is proportional to the mean solvated molecular volume u,":
[ q ] * M = 2.5Nou, (4)
where No is the Avogadro constant. The molecular size calculation can be applied to PEG oligomers, for which the intrinsic viscosity-molecular weight relationship is known. A calibration of the SEC columns is obtained in the form of a time of retention-molecular size relationship. Applying this relation to the SEC spectra for PF enables one to obtain the molecular size distribu- tion of the PF in a given solvent system, Thus, a measure of the molecular size is obtained, enabling one to make size comparisons of the macromolecules in different solvents. This is not possible when calibration is conducted using M only.
Specifically, using the MH parameters, or an empiric quadratic relation such as
log[q] = A + B log(A4) + C log(M)2 where A, B, and C are constants (Table I), to calibrate the PEG molecular
LOW MW POLY(ETHYLENE OXIDE) AND PF RESOLS 347
al ul C 0 ul a E L
c 0 V 0 al CI
100 1000 1 E4- Molecular weight (g -mo l ' )
Fig. 3. Molecular weight and molecular size, [ q ] M , distribution for a spray-dried resin in tetrahydrofuran with 0.4% trifluoroacetic acid at 25C determined with Ultrastyragel 100 and 500 A columns in series.
weights in terms of molecular size [ v], ([ 171 * M ) values are calculated for the resols in the different solvent systems mentioned and a molecular size distri- bution is calculated form elution data. These a...